| ||Format||Pages||Price|| |
|9||$52.00||  ADD TO CART|
|Hardcopy (shipping and handling)||9||$52.00||  ADD TO CART|
Significance and Use
4.1 The procedures given are designed to remove corrosion products without significant removal of base metal. This allows an accurate determination of the mass loss of the metal or alloy that occurred during exposure to the corrosive environment.
4.2 These procedures, in some cases, may apply to metal coatings. However, possible effects from the substrate must be considered.
1.1 This practice covers suggested procedures for preparing bare, solid metal specimens for tests, for removing corrosion products after the test has been completed, and for evaluating the corrosion damage that has occurred. Emphasis is placed on procedures related to the evaluation of corrosion by mass loss and pitting measurements. (Warning—In many cases the corrosion product on the reactive metals titanium and zirconium is a hard and tightly bonded oxide that defies removal by chemical or ordinary mechanical means. In many such cases, corrosion rates are established by mass gain rather than mass loss.)
1.2 The values stated in SI units are to be regarded as standard. No other units of measurement are included in this standard.
1.3 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety, health, and environmental practices and determine the applicability of regulatory limitations prior to use. For specific warning statements, see and .
1.4 This international standard was developed in accordance with internationally recognized principles on standardization established in the Decision on Principles for the Development of International Standards, Guides and Recommendations issued by the World Trade Organization Technical Barriers to Trade (TBT) Committee.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
A262 Practices for Detecting Susceptibility to Intergranular Attack in Austenitic Stainless Steels
D1193 Specification for Reagent Water
D1384 Test Method for Corrosion Test for Engine Coolants in Glassware
D2776 Methods of Test for Corrosivity of Water in the Absence of Heat Transfer (Electrical Methods)
G16 Guide for Applying Statistics to Analysis of Corrosion Data
G31 Guide for Laboratory Immersion Corrosion Testing of Metals
G33 Practice for Recording Data from Atmospheric Corrosion Tests of Metallic-Coated Steel Specimens
G46 Guide for Examination and Evaluation of Pitting Corrosion
G50 Practice for Conducting Atmospheric Corrosion Tests on Metals
G78 Guide for Crevice Corrosion Testing of Iron-Base and Nickel-Base Stainless Alloys in Seawater and Other Chloride-Containing Aqueous Environments
ICS Number Code 77.060 (Corrosion of metals)
UNSPSC Code 41114604(Corrosion testers)
|Link to Active (This link will always route to the current Active version of the standard.)|
ASTM G1-03(2017)e1, Standard Practice for Preparing, Cleaning, and Evaluating Corrosion Test Specimens, ASTM International, West Conshohocken, PA, 2017, www.astm.orgBack to Top